Proceedings of the 12th International Conference on Aluminium Alloys, September 5-9, 2010, Yokohama, Japan ©2010 The Japan Institute of Light Metals pp. 2120-2124 2120 Investigation of Non-isothermal Aging process of 7085 Aluminum Alloy K. Li1, K. Zhang2, L. Yang1, J. Z. Chen2 and L. Zhen1 1 School of Materials Science and Engineering, Harbin Institute of Technology, Harbin 150001, China 2 Beijing Institute of Aeronautical Materials, Beijing 100095, China Non-isothermal aging (NIA) process of 7085 aluminum alloy was investigated in the current study aiming to obtained good performance combinations through hardness measurement, conductivity measurement and microstructure characterization. The hardness of peak-aged 7085 alloy was observed to slightly affected by the starting temperature as well as the heating rate, which then suggested a wide process scope of non-isothermal aging. The non-isothermal aged 7085 alloy presents high strength as well as high SCC resistance. Specifically, a tensile strength of 524 MPa, an yield strength of 506 MPa, an elongation of 14.2% and an electriccal conductivity of 40%IACS were obtained in NIAed 7085 aluminum alloy of over-aged state, which was near to that obtained through T74 treatment. Additionally, very weak anisotropy was observed in mechanical performances of forged thick plate, which was beneficial for manufacturing huge and muti-way bearing components. TEM observation suggested that the over-aged microstructure of NIAed 7085 alloy was similar to that observed in 7085-T74 specimen. Keywords: Aluminum alloy, non-isothermal aging, mechanical performance, SCC resistance 1. Introduction To displace builtup structures with large forgings is an effective way to promote the integral manufacture in the field of airspace . Besides forge process, the post-forming heat-treatment is also a crucial step for obtaining high performance, especially for aging hardenable aluminum alloys. The large size of forgings however hinders the performing of usual isothermal aging process, because to heat or to cool large forgings quickly and uniformly is rather difficult. Non-isothermal aging (NIA) processes thus become imperative for this series of applications since the microstructure tailoring is crucial for performance control . Previous study suggested that aluminum alloy of 7000 series should be applied at over-aged state, such as T74, T76 ,T77 and RRA state, to obtain high SCC resistance and high toughness at cost of strength . Among these processes, RRA compromises properly between strength and other two performances by introducing retrogression step, which was quite effective to enhance GB precipitation and simultaneously suppress the growth of intragranular precipitations. The typical microstructure of aluminum alloy treated through RRA process, including dispersed GB precipitations and fine intragranular precipitations, was thought to beneficial for obtaining high SCC resistance at low cost of strength [4,5]. To avoid the complicated and time-consuming experimental, SCC resistance of aluminum alloys was usually indirectly evaluated through conductivity measurements in many works [6, 7], which was believed to be an effective method. 7085 aluminum alloy is a preferred material for large forgings used in load-carrying components in aircraft for its excellent through-quenching property, high mechanical performance and high SCC resistance . However, experimental study on the non-isothermal aging of 7085 aluminum alloy is now quite limited [8-11] and how to obtain good performances including high toughness, high SCC resistance and high strength remains unclear. The current study was thus inspired to investigate the aging behavior of 7085 aluminum alloy during non-isothermal aging. The attention was focused on the strength and SCC resistance. 2121 2. Experimental Forged and tempered thick plate of 7085 aluminum alloy was used as raw materials in the current study and the chemical composition of the alloy was shown in Table 1. Specimens for hardness measurement and tensile measurement were cut from the raw plate, solid soluted at 470 oC for 2 h and water quenched to room temperature. Immediately after quenched, these specimens were iso-thermal aged at processes with heating rate (Rh) of 5, 10 and 20 oC/h from starting temperature (Ts) of 20 oC and 120 oC respectively. Brinell hardness was then measured with a load of 7350 N and a load holding time of 30 seconds. Tensile test of some specimens was performed on an Instron testing machine at room temperature. The evaluation of SCC resistance was performed indirectly through conductivity measurements on strip specimens 1×1×40mm in size, with reference to the previous work . Microstructure of a few specimens was observed on TEM (Philips, Tecnai 20). Table 1 Chemical composition of 7085aluminum alloy (wt.%) Element Zn Mg Cu Zr Fe Si Ti-B Al Content 7.67 1.69 1.75 0.12 0.026 0.013 0.0022 Balance 3. Results and discussion Dependence of hardness on time in 7085 aluminum alloy during NIA treatment was demonstrated in Fig.1. It was apparent that, hardening behavior observed at various processes was similarly to each other: hardness increased gradually to peak values and then decreased quickly. The quick decrease of hardness observed here was attributed to the accelerated coarsening of precipitations driven by the persistently raised temperature. The temperature of isothermal aging of 7000 series aluminum alloy is usually no higher than 160 oC, the much higher temperature in the later stage of NIA in current processes thus led to much higher coarsening rate and quick softening, similar phenomenon was previously observed in 7000 aluminum alloy [12, 13]. Variation of conductivity of 7085 aluminum alloy during NIA was demonstrated in Fig. 2, from which a slightly accelerative increase of conductivity can be observed in various processes. It was thought the knee position at about 150 oC resulted from the massive precipitation of η ' phase. It was also found that, Ts affected the conductivity very slightly at very Rh condition. However, conductivity was found to be lower when higher Rh, was applied, which we thought was related to less insufficient precipitation resulted from the shorter process duration. 190 (a) 190 (b) 180 180 170 170 170 160 160 160 150 150 150 140 o o Ts=20 C, 5 C/h 120 Ts=120 C, 5 C/h o 3 6 9 o 12 15 18 21 24 27 30 33 36 39 42 Time/h 130 o o Ts=20 C, 10 C/h o o Ts=120 C, 10 C/h 120 110 (c) 140 140 130 110 0 HB 180 HB HB 190 0 3 6 9 12 Time/h 15 18 21 o o o o 130 Ts=20 C, 20 C/h 120 Ts=120 C, 20 C/h 110 0 3 6 Time/h 9 12 Fig.1 Dependence of Brinell hardness on time in7085 aluminum alloy during NIA with Rh of (a) 5 C/h, (b) 10oC/h and (c) 20oC/h o 2122 46 48 (a) 46 Conductivity/%IACS Conductivity/%IACS 46 44 44 42 40 38 36 34 Ts=20 C, 5 C/h 32 Ts=120 C, 5 C/h 30 28 48 (b) 130 140 150 160 170 180 o Temperature/ C o o o o 190 200 42 40 38 36 o o 34 Ts=20 C, 10 C/h 32 Ts=120 C, 10 C/h o o 30 210 28 Conductivity/%IACS 48 (C) 44 42 40 38 36 34 140 150 160 170 180 o Temperature/ C 190 200 210 28 o o o 190 200 Ts=120 C, 20 C/h 30 130 o Ts=20 C, 20 C/h 32 130 140 150 160 170 180 o Temperature/ C 210 Fig. 2 Dependence of conductivity on temperature of 7085 aluminum alloy during NIA with Rh of (a) 5oC/h, (b) 10oC/h and (c) 20oC/h The detailed parameters of process as well as performance in cases of peak aged state were derived from curves demonstrated in Fig. 1 and Fig. 2 and listed in Table 2, which can demonstrate more precisely the effect of parameters. Hardness as well as conductivity of peak-aged 7085 aluminum alloy treated through various NIA processes was very similar to each other, which suggested that Ts as well as Rh did not influence the performance significantly in a wide scope. However, the process parameters were found to apparently affect the time and temperature at which a peak-aged state was obtained. As shown in Table 2, temperature increased but time decreased with Rh, at cases of either Ts, which was due to the effect of temperature on precipitation rate. When higher Rh, applied, temperature rise more quickly and precipitation can be accelerated, peak aged state thus can be obtained earlier. On the other hand, increase of Ts from 20 oC to 120 oC was found to greatly shorten the time need to reach peak-aged state with no effect on temperature, indicating that precipitation can hardly occur when 7085 aluminum alloy was heat-treated at temperatures lower than 120 oC. Process Rh Ts (oC/h) (oC) 5 20 10 20 5 120 10 20 Table 2 Parameters of peak-aged situation Parameters of peak aged state Time Temperature Conductivity HB (h) (oC) (%IACS) 36.1 28 160 187 15 170 187 36.8 8 180 186 36.8 36.0 8 160 187 5 170 187 36.5 3 180 188 36.9 As discussed above, high Rh, as well as high Ts was beneficial for aging efficiency with slight effect on performance, thus Rh, of 20 oC/h and Ts of 120 oC was applied to heat-treat tensile specimens for verification. The obtained tensile performance in both L and LT direction was shown in Fig.3. The peak-aged state was obtained at temperature of 180 oC, which was consistent to that derived from hardness measurement. Typically, yield strength of 515 MPa, tensile strength of 550 MPa and elongation of 14% can be obtained in 7085 aluminum alloy of peak aged, which was near to that previously obtained at T74 state. Notably, a rather high yield/tensile ratio was observed in 7085 aluminum alloy at peak-aged as well as over-aged state, which was beneficial for exerting the intensity potential of this alloy. It was also found that, the performance measured in two directions were near to each other and the forged plated was nearly isotropic, which is important for large forgings bearing multiway-load, such as the tail girder in aircrafts. 2123 600 48 550 44 40 450 σb,L 400 σb,L-T 350 σs,L 36 32 28 σs, L-T 300 24 δ, L δ, L-T 250 200 20 16 150 100 δ/% Tensile strength/MPa 500 12 140 150 160 170 o 180 190 200 Temperature/ C Fig.4 Tensile performance of 7085 aluminum alloy of different state, Rh,=20oC, Ts=120 oC However, SCC resistance of peak-aged 7085 aluminum alloy was thought to be low as the corresponding conductivity was lower than 37 %IACS. With reference of previous study on 7000 aluminum alloy, conductivity as high as 40%IACS was believed to be an indication of high SCC resistance , which can be obtained at over-aged 7085 aluminum alloy in the current study. Typical performance of over-aged 7085 aluminum alloy treated through NIA process were shown in Table 3, which was similar to that obtained through the typical T74 process. Table3 Typical performances obtained in non-isothermal aged 7085 aluminum alloy, Rh,= 20oC, Ts=120 oC Temperature Conductivity σ0.2 σb δ Orientation Hardness (oC) (%IACS) (MPa) (MPa) (%) L 512 476 14 HB165 200 41.2 L-T 510 474 13.2 L 529 487 13.6 HB173 195 40 L-T 523 485 13 The typical morphology of NIAed 7085 aluminum alloy of different state was observed on a TEM and typical images were shown in Fig.5. Very fine precipitations were observed to shape up and diffraction contrast between matrix and precipitation was weak, indicating an under-aged state. When heated to 140 oC. When heated to 180oC, more precipitations with larger size were observed in grains and some coarsened particles appeared on GBs. When heated further to 200 oC, intragranular precipitations coarsened greatly to about 40 nm and the the precipitation on GBs become isolated from each other, which was similar to that observed in specimens of T74 state. Fig.5 TEM morphology of NIAed 7085 aluminum alloy of different state quenched at (a) 140 oC, (b) 180oC, and (c) 200 oC 2124 4. Conclusions Non-isothermal aging process was preliminary investigated concerned in the requirement from post-age heat-treatment of large components in aircrafts. Specifically, effect of starting temperature (Ts) and heating-rate (Rh,) on mechanical performance and SCC resistance was systematically investigated based on measurement of hardness and conductivity. It was found that, Ts, Rh, affected hardness and conductivity of peak-aged 7085 aluminum alloy very slightly in a wide range, which then provide a broad process window for post-forge aging. Additionally, high Ts and high Rh contributed to high process efficiency, as observed in the study. Tensile test suggested that, high performance could be obtained through NIA process. Specifically, a tensile strength of 524 MPa, yield strength of 506 MPa, an elongation of 14.2% and an electric conductivity of 40%IACS were obtained, which was similar to that obtained through T74 process. High isotropy of mechanical performances and high yield/tensile ration was observed in the NIAed 7085 aluminum alloy, which was critical for application in components bearing multi-way load in air crafts. References      J. C. Williams, E. A. Starke Jr: Acta Mater, 51(2003) 5775-5799. C. R. Hutchinson, M. Goune, A. Redjaimia: Acta Mater. 55(2007) 213-223. E. A. Starke and J. T. Staley: Aerospace Sci. 32 (1996) 131-172. BM Cina: US Patent 3856584 (1974). A. F Oliveira Jr. , M.C de Barros , K. R Cardoso and D. N Travessa: Materials Science and Engineering: A. 379(2004) 321-326.  P. Guyot and L. Cottignies: Acta Mater. 44(1996) 4161-4167.  F. Andreatta, H. Terryn and J. H. W. de wit: Electrochimica Acta, 49(2004) 17-18.  Myriam Nicolas and Alexis Deschamps: Acta Mater. 51(2003) 6077-6094.  James T. Staley: US patent 20070267113Al. I. N. Khan and M. J. Starink: Materials Science and Technology, 24(2008) 1403-1410. C. R. Hutchinson, M. Goune, A. Redjaimia: Acta Mater. 55(2007) 213-223. Z. W. Du, Z. M. Sun, B. L. Shao, T. T. Zhou and C. Q. Chen: Materials Characterization, 56(2006) 121-128. M. J. Starink and S. C. Wang: Acta Mater, 51(2003) 5131-5150.